Masterbatch Gb 2013
Embed Size (px)
Transcript of Masterbatch Gb 2013
LEISTRITZ EXTRUSIONSTECHNIK GMBH
r e f r e s h i n g e x t r u s i o n t e c h n o l o g y
2Masterbatch - Small, but with Great Effect
Masterbatch - the Grain of Difference
Polymer granulates with a high percentage of additives, higher than in the end use, are called masterbatch. In later production steps, such as injection moulding, film or fibre production, those granulates are mixed with the raw polymer for colouring or the targeted modification of certain properties.
Advantages: In comparison to pastes, powders or fluid additives, using masterbatch increases the process stabi-lity. The reason lies in the exactly defined pigment quantity in each granulate. Additionally: Since there is no handling of large powder masses and therefore the environment and the work station are not being polluted, masterbatch is regarded to be a very good processing material.
Raw polymer> 10%
Pigments Organic pigments Inorganic pigments Effect pigments Monobatches
Additives Heat stabilizers Light stabilizers Flame retardants Antistatics Antiblock agents Nucleating agents
Fillers Fillers Reinforcers
Generally, there are three masterbatch groups:
1. Colour masterbatch, which is used for colouring plastics products 2. Additive masterbatch, which provides for certain chemical and physical properties of the end product (for example UV stabilizers, flame retardants, antistatics or antiblock agents) 3. Filler masterbatch, that is filled with a high share of fillers like chalk
Films / Panels
* see pages 6-9
Particle shapeDust formationDispersibilityColour strengthResist. to shape distortionResistance to migrationProcessibility
0.01 0.1 m
more dispersing energy needed, difficult
premix- and split-feed* possible
1 20 m
little shearing, easy to disperse, sometimes
premix- and split-feed* possible
2 180 m
step chipsn. s.n. s.n. s.n. s.n. s.
shear sensitive - as little shear forces as possible, as
high mixing effect as possible
very uneven: ranging from very small to large
depending on the pigment ++
++(+)depending on the pigment depending on the pigment depending on the pigment fully dispersed, hardly any shearing needed, melted
The goal of masterbatch production is the ideal dispersion of additives in the polymer matrix. The fine, powdery feed material often tends to agglomerate and therefore is difficult to work with. Masterbatches with an additive share of 20 - 90% are available, depending on the feed material.
The co-rotating twin screw extruder is the heart of a masterbatch line. High dispersion efficiency and self-cleaning are factors that are crucial for masterbatch production. The products comply with the highest demands in quality, as for example required in the production of synthetic fibres.
ZSE 40 MAXX - ideal for masterbatch production with throughputs of up to 500 kg/h (depending on the application)
Dispersive & Distributive Mixing
Dispersion is the incorporation of pigments, additives or fillers into a binder or carrier. This process is divided into four steps:
1. wetting of the pigments/additives/fillers2. splitting of the agglomerates (dispersive mixing)3. distribution of the pigments/additives/fillers in the melt (distributive mixing)4. stabilization against re-agglomeration
nThe basic function of distributive mixing is the distribu-tion of the material without destroying the single com-ponents. Distributed particles can be elongated further in order to achieve a more even distribution of the mor-phological components.
There are two different methods for producing masterbatch, the single-stage process and the two-stage pro-cess.
Here, all of the components in the concentrate are combined in one processing step. The process can be rea-lized either via a premix setup (only one feeder above the main opening port) or via a split-feed setup, where each component is fed into the extruder by means of a feeder positioned above the main feed port and one or two side feeders. The single-stage process is applied for all three masterbatch groups.
In this process, which is applied only for the production of colour masterbatch, single pigment concentrates are produced in the same manner as in the one-stage process. The first step is then followed by a second extrusion step that combines the required ratios of colourant and additive single pigment concentrate to create a master-batch which is customized to the specifications of the customer.
Single-Stage Masterbatch Production
Two-Stage Masterbatch Production
Custom Colouring Phase 2
Twin screw extruder
Feeding of all raw material
Pelletization of the single pigment
Twin screw extruder
Feeding of a colourant and a carrier matrix
Feeding of single pigment concentrates
Single or twin screw extruder
Strand or underwater pelletization
Comparison of Production Processes
40% LLDPE powder40% pigment blue 15:320% Wax
1200 rpm 280 kg/h
900 rpm 190 kg/h
600 rpm 95 kg/h
Masterbatch quality also depends on the choice of the premix process. Comparison of hot and cold mix on the basis of a certain application
Example of Use
* see page 11
In this case, better values are achieved with the hot mix, since here the pigments are wetted with wax.
ZSE 50 MAXX line for processing a premix
Adding of material via main feed port
Adding of material via at least two feeders in various feed ports
Without waxWith waxCold mixHot mix
Overview: Impact of Process Engineering on Colour Masterbatch Production
Wax / pigmentpremix
Wax / pigmentseparate feeding
When using this, most widely spread production process, a premix consisting of polymer, pigment and disper-sion additives is fed to the extruder. Normally, these premixes are produced in batches in a previous mixing step. Great importance must be given to this premix process. If a mistake happens here, unfortunately, oftentimes it is very difficult to make corrections during the extrusion step. Due to the usage of volumetric feeders, there is a high operational reliability, handling is quite uncomplicated, and the process is very popular as well as low priced.
The finished premix is fed into the extruder via a volumetric feeder. The extruder takes on the part of homogenizing and dispersion, wetting as well as distributing the pigments in the polymer matrix. In most cases a common strand granulation system is used.
Volumetric dosing unit
In this version of masterbatch production, the polymer is plastified first. Then the other formulation components (pigments, fillers and if needed dispersion aids) are added via one or two side stuffers (hot melt extrusion). Feeding is done via separate gravimetric feeders. The handling of the formulation via the extruder or feed control is rela-tively uncomplicated and does not need elaborate premixing. This makes big scale masterbatch production much easier.
Incorporation of Effect Pigments: Split-Feed is More Gentle than Premix
When processing sensitive pigments (such as organic or effect pigments) split-feed is the right choice, because with this setup the pigments are incorporated into the melt more gently, and therefore experience less shearing. Split-feed must also be used when feeding a very high share of additives, since the according quantity of material cannot be fed only via the main feed port. The material stream is then divided.
Split-feed, ZSE MAXX Premix, ZSE MAXX
Mica based effect pigment in a polymer matrix: Larger particles in split-feed application better quality.
Container with pigment
Degassing / Vacuum
Gravimetric feeder for dispersion aidsGravimetric feeder
Ideal for colour sampling or low-scale production in continuous operation: ZSE 18 MAXX (200 g/h - 40 kg/h) - scale-up is possible
ZSE 50 MAXX with split-feed